General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.82 g/cm³ Show Material materials with Density of 7.82 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation | 20.0 °C | 20 - 22 % Show Material materials with Elongation of 20 - 22 % | |

Elongation, transverse | 20.0 °C | 12 - 15 % Show Material materials with Elongation, transverse of 12 - 15 % | |

Poisson's ratio | 23.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | Typical for Medium Carbon Steel |

Shear modulus | 23.0 °C | 75 - 80 GPa Show Material materials with Shear modulus of 75 - 80 GPa | Typical for Carbon Steel |

Tensile strength | 20.0 °C | 490 - 610 MPa Show Material materials with Tensile strength of 490 - 610 MPa | |

Tensile strength, transverse | 20.0 °C | 490 - 610 MPa Show Material materials with Tensile strength, transverse of 490 - 610 MPa | |

Yield strength | 20.0 °C | 245 - 275 MPa Show Material materials with Yield strength of 245 - 275 MPa | |

Yield strength, transverse | 20.0 °C | 245 - 275 MPa Show Material materials with Yield strength, transverse of 245 - 275 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | ||

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Melting point | 1380 - 1514 °C Show Material materials with Melting point of 1380 - 1514 °C | Typical for Medium Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 48 W/(m·K) Show Material materials with Thermal conductivity of 48 W/(m·K) | |

100.0 °C | 48.9 W/(m·K) Show Material materials with Thermal conductivity of 48.9 W/(m·K) | ||

200.0 °C | 47.5 W/(m·K) Show Material materials with Thermal conductivity of 47.5 W/(m·K) | ||

300.0 °C | 44.7 W/(m·K) Show Material materials with Thermal conductivity of 44.7 W/(m·K) | ||

400.0 °C | 41.6 W/(m·K) Show Material materials with Thermal conductivity of 41.6 W/(m·K) | ||

500.0 °C | 38.6 W/(m·K) Show Material materials with Thermal conductivity of 38.6 W/(m·K) | ||

600.0 °C | 35.5 W/(m·K) Show Material materials with Thermal conductivity of 35.5 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 13.3 mm²/s Show Material materials with Thermal diffusivity of 13.3 mm²/s | |

100.0 °C | 12.6 mm²/s Show Material materials with Thermal diffusivity of 12.6 mm²/s | ||

200.0 °C | 11.5 mm²/s Show Material materials with Thermal diffusivity of 11.5 mm²/s | ||

300.0 °C | 10.2 mm²/s Show Material materials with Thermal diffusivity of 10.2 mm²/s | ||

400.0 °C | 8.9 mm²/s Show Material materials with Thermal diffusivity of 8.9 mm²/s | ||

500.0 °C | 7.5 mm²/s Show Material materials with Thermal diffusivity of 7.5 mm²/s | ||

600.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2.17E-7 Ω·m Show Material materials with Electrical resistivity of 2.17E-7 Ω·m |

100.0 °C | 2.62E-7 Ω·m Show Material materials with Electrical resistivity of 2.62E-7 Ω·m | |

200.0 °C | 3.32E-7 Ω·m Show Material materials with Electrical resistivity of 3.32E-7 Ω·m | |

300.0 °C | 4.2E-7 Ω·m Show Material materials with Electrical resistivity of 4.2E-7 Ω·m | |

400.0 °C | 5.23E-7 Ω·m Show Material materials with Electrical resistivity of 5.23E-7 Ω·m | |

500.0 °C | 6.41E-7 Ω·m Show Material materials with Electrical resistivity of 6.41E-7 Ω·m | |

600.0 °C | 7.8E-7 Ω·m Show Material materials with Electrical resistivity of 7.8E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.32 - 0.39 % Show Material materials with Carbon of 0.32 - 0.39 % |

Chromium | 0.4 % Show Material materials with Chromium of 0.4 % |

Manganese | 0.5 - 0.8 % Show Material materials with Manganese of 0.5 - 0.8 % |

Molybdenum | 0.1 % Show Material materials with Molybdenum of 0.1 % |

Nickel | 0.4 % Show Material materials with Nickel of 0.4 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % |

Sulfur | 0.035 % Show Material materials with Sulfur of 0.035 % |